Like this document? Why not share!

- C:\Documents And Settings\Ch13897\D... by guest87dcd7 566 views
- Design of aluminium structures for ... by StroNGER2012 206 views
- Numerical modeling of the welding d... by inventy 267 views
- Report_Modified_1 by Muhassin Nijumudheen 45 views
- shoaib_CV-28-8-15 by Mohammed Shoaib T... 205 views
- Bs5950 1-structural use of steelwor... by onyejekwe 7477 views

2,011

-1

-1

Published on

Published in:
Education

No Downloads

Total Views

2,011

On Slideshare

0

From Embeds

0

Number of Embeds

0

Shares

0

Downloads

179

Comments

0

Likes

1

No embeds

No notes for slide

- 1. TALAT Lecture 2402 Design Recommendations for Fatigue Loaded Structures 60 pages, 36 figures Advanced Level prepared by Dimitris Kosteas, Technische Universität München Objectives: − Calculation of design stresses for variable stress ratios in practice, explanation on the background of design recommendations − To teach the concept of partial safety factors and supply appropriate background information for aluminium − To enable the designer to evaluate service behaviour of structural details on a more sophisticated level applying the same principles as in current design recommendations − To provide understanding of the fatigue design procedure according to current recommendations Prerequisites: − Background knowledge in engineering, materials and fatigue as well as some knowledge in statistics required Date of Issue: 1994 © EAA - European Aluminium Association TALAT 2402 1
- 2. 2402 Design Recommendations for Fatigue Loaded Structures Table of Contents 2402 Design Recommendations for Fatigue Loaded Structures................................2 2402.01 The R-Ratio Effect ...................................................................................... 4 Data Background......................................................................................................5 Data Evaluations ......................................................................................................5 Stage II Evaluation ............................................................................................... 7 Stage III Evaluation .............................................................................................. 9 Drafting a Proposal for the Factor f(R)..................................................................13 Final ERAAS Design Proposal for f(R).................................................................15 Residual Stress Effects...........................................................................................16 Appendix................................................................................................................18 2402.02 Safety and Reliability................................................................................ 19 Reliability Concept ................................................................................................19 Partial Safety Factor Concept ................................................................................23 Concept of Fatigue Design Curves ........................................................................25 2402.03 Background on Current Design Recommendations .............................. 26 European Recommendations ERAAS Fatigue Design 1992 .................................26 Full-Size Component Testing and Analysis ........................................................ 27 Detail Classification and Design Curves............................................................ 32 The S-N Slope Proposal ...................................................................................... 33 Comparison to Steel Codes................................................................................. 35 The British Standard 8118: 1991 ..........................................................................38 Data Sources....................................................................................................... 39 Data Analysis and Detail Classification............................................................. 41 Design Curves..................................................................................................... 42 Classification of Details...................................................................................... 42 Comparison between ERAAS and BS 8118..........................................................43 TALAT 2402 2
- 3. 2402.04 Fatigue Design Calculation Example: Gusset Plate Welded on Edge of Tubular Element ....................................................................................................... 47 Design Procedure ...................................................................................................47 Calculation Example after ERAAS .......................................................................49 Loading ............................................................................................................... 50 Classification of Structural Detail...................................................................... 50 Fatigue Assessment............................................................................................. 50 Concluding Remarks........................................................................................... 52 Utilising the TUM-ALFABET Software ...............................................................53 Calculation Example after BS 8118.......................................................................53 Loading ............................................................................................................... 54 Classification of Structural Detail...................................................................... 54 Fatigue Assessment............................................................................................. 55 Concluding Remarks........................................................................................... 56 Literature References for Lecture 2402.04 ............................................................57 2402.05 Literature/References ................................................................................. 58 2402.06 List of Figures.............................................................................................. 59 TALAT 2402 3
- 4. 2402.01 The R-Ratio Effect • Data background • Data evaluations • Drafting a proposal for the factor f(R) • Final ERAAS design proposal for f(R) • Residual stress effects Assumptions and statements made in the following are based on information and experi- mental test data available in connection with the ECCS-EAA Fatigue Workshops in Munich and Zurich in February and March 1990, respectively. These intermediate results helped to formulate the outline of R-ratio effects presented. Due to the succeeding discussions in the ECCS Committee 2 concerning the drafting of the European Recommendations for Aluminium Alloy Structures in Fatigue Design (ERAAS Fatigue) in meetings in the following summer and winter, as well as due to further intensive evaluations and the enforcement of general principles governing the format of fatigue design procedures, the final R-ratio dependency of fatigue strength design values is not always identical to the first actual results. There is, unfortunately, incomplete experimental information to allow a quantitative statement on the effect of R-ratio on the fatigue strength of aluminium structural elements. Accordingly the treatment of this effect has varied in the past with the data available or reflecting the viewpoint of those drafting the respective recommendation, see Figure 2402.01.01. Aluminium Fatigue Design Recommendations R-independent R-dependent DVS 1608 (1969) "LDV" (1970) ALCAN Handbook UNI 8634 (12/1985) Austrian Recommendations (3/1988) Assoc. American RR Freight Cars (3/1980) Ontario Highway Bridge Code (1979/1983) Recommended Specifications Aluminium Association (10/1985) BS 8118: (1985) light/heavy struct. el. (1989) ERAAS Fatigue Design up to Draft 8:1985 ERAAS Fatigue Design, Doc. 68, 1992 Source: D. Kosteas, TUM alu Training in Aluminium Application Technologies R-Dependencies in Fatigue Design Recommendations 2402.01.01 Roughly, earlier recommendations accept R-dependent fatigue strength values, since they seem to be based either on small specimen test results, or on rather simple TALAT 2402 4
- 5. structural elements or even only on base material with no significant residual stresses. More recent fatigue design rules, in steel as well as in aluminium, attempt to place the emphasis on the behaviour of larger, full-size components and welded constructions and thus assume the presence of more or less significant residual stresses. Consequently, the latter are based on a R-ratio-free design concept and do not always make use of any possible beneficial effect for R values near or below zero. Although not explicitly stated, it can be derived from respective experimental evidence that fatigue strength values at approximately R = + 0.5 or higher have formed the basis of the proposed design values. The fact that the ERAAS-Fatigue Design values are given both as R-independent and R- dependent reflects the growing knowledge level during the drafting period of the re- commendations and the desire to cover possible beneficial structural cases. Data Background The first comprehensive data evaluation attempt in 1985-1986 was confined to analysis of fatigue tests with small specimens only, the so-called CAFDEE test data. During the second data evaluation stage interest focused on larger components, the welded and base material beam fatigue tests performed by the TUM and earlier respective tests made available by the aluminium industry. Again comparative analysis of fatigue tests at two different R-values were possible with the beam test results from TUM only. A set of small specimen data at different R levels was analysed in parallel, though, allowing for a comparison along the lines of this homogeneous data a comparison with earlier assumptions in analyses and recommendations. The decision was taken at this stage to refrain from attempting a quantification of the R-ratio effect on fatigue strength and operate along the assumption of larger structural elements with respective significant residual stresses and consequently adopt an R-independent design procedure. Discussions that followed on the next ECCS TC2 meeting in Grenoble in November 1989 and different reactions to the above proposal prior to and during the third comprehensive data evaluations at the EAA-ECCS Fatigue Workshops in Munich, February 1990, and Zurich, March 1990, now encompassing the more recent test results of the second TUM beam fatigue test program and a new large contingent of further test data on small specimens made available by the aluminium industry, expressed the wish for a better differentiation of cases possible in practice. Information on R-dependency was summarised once more, opening the possibility to the design engineer to distinguish between more cases in practice and utilise beneficial effects where this would seem appropriate. Data Evaluations Information on the data analysed on the three mentioned evaluation stages is summarised: Stage I: Due to the non-homogenous character and the unreliability in the documentation of earlier test data it was decided not to use the old material for purposes of the European recommendations. TALAT 2402 5
- 6. Stage II: (a) Type: ALS (Alusuisse/Zurich resp. Neuhausen) small speci- mens, 6005A alloy base metal, transverse butt weld Sample size: 424 and 407 respectively typical data set sample size: 41 Life range: 104 to 2.106 cycles R-ratio: values between -3 and +0.7 Information: see Fig. 4 and Fig. 5 EAA-Report March 1989 (b) Type: TUM beams, 7020 alloy transverse butt weld, longitudinal and transverse fillet weld attachment on beam flange Sample size: total/at R=0.1/at R=-1 butt weld 43/23/15 long. fillet attach. 53/19/34 transv. fill./cover plate 43/15/28 Life range: . 6 10 4 to 2.106 cycles R-ratio: values for -1 and +0.1 Information: EAA Report 3/89 Stage III: (c) Type: TUM beams in 7020 and 6005A alloys, due to the still running tests of the 1987-1990 test series at the time of these evaluations and the resulting small sample sizes only a limited number of cases give valid statements Sample size: web-to-flange fillet welds 87 cover plate 26 Life range: 104 to 5.106 cycles R-ratio: -1, +0.1, +0.6 Information: Fatigue Workshop Munich,1990 (d) Type: small specimens, different structural details and alloys of the 5000/6000/7000 series Sample size: base metal 7020 : 2209 5000 : 1719 6000 : 5035 notches, holes : 851 butt weld : 6027 web stiffener or non-load-carr. transv. fillet : 1586 cruciform or load-carrying transv. fillet : 1262 Life range: 104 to 107 cycles R-ratio: -1 and +0.1 Information: Fatigue Workshop Documents, 1990 Alusuisse Zurich data TALAT 2402 6
- 7. Stage II Evaluation The relationship in Figure 2402.01.02 is based on mean fatigue strength values at one million cycles estimated by linear regression analysis, excluding run-outs. During the Munich Workshop though, a second relationship, with somewhat different values, was established, this one based on lower boundary curves for the test data at two million cycles: R -3 -2 -1 -0,5 0/0,1 +0,3 +0,5 +0,7 SR 166 166 166 129 113 96 86 79 [MPa] SR/S0.5 1,93 1,93 1,93 1,50 1,31 1,12 1,00 0,92 estimated mean at 106 300 250 Fatigue Strength 200 190 -> 1.61 150 142 -> 1.20 118 -> 1.00 100 50 -4 -3.5 -3 -2.5 -2 -1.5 -1 -0.5 0 0.5 1 R-Ratio alu R-Ratio vs. Fatigue Strength Training in Aluminium Application Technologies for Base Metal Small Specimen Test Data 2402.01.02 This was considered more representative and was used (at this stage of development) to establish the fatigue strength enhancement factor f(R) in the case of base material, see further on Figure 2402.01.04. It is mentioned at this point already that the respective value stated on the first column of Figure 2402.01.06 has been derived directly from the figures of the above table. Concerning information on the transverse butt weld specimens again as mean stress values at one million cycles the relationship of Figure 2402.01.03 is established. TALAT 2402 7
- 8. estimated mean at 106 210 190 170 Fatigue Strength 150 133 -> 1.75 130 110 95 -> 1.25 90 76 -> 1.00 70 50 -4 -3.5 -3 -2.5 -2 -1.5 -1 -0.5 0 0.5 1 R-Ratio alu R-Ratio vs. Fatigue Strength Training in Aluminium Application Technologies for Transverse Butt Weld Small Specimen Fatigue Data 2402.01.03 Or, again, the following relationship if strength values at two million cycles are used: R -3 -2 -1 -0,5 0/0,1 +0,3 +0,5 +0,7 SR 131 131 76 (95) 54 54 50 46 [MPa] S-1/S+0,5 = 1.52 S-1/S0 = 1.41 Initially it was thought that both, base material and (butt) welded joints, could be treated by a common assumption due to the factors originating from Figure 2402.01.02 and Figure 2402.01.03 with data from small specimen tests. Comparison of different data exhibited different fatigue strength ratios at respective R values and there was no clear overall picture. Some of this information will be given in the following. The proposal thus for welded details, according to Figure 2402.01.04, assumes a relationship parallel to the one for base material but on a lower level. The characteristic f(R) value at R = -1 equals 1.6 and reaches 1 for R = 0, being thus on the safe side. TALAT 2402 8
- 9. Factor f(R) 1.9 I. 1.6 II. 1.3 I - II 1 -1 -0.5 0 0.5 1 R-Ratio I. Base Metal II. Butt Weld Source:D. Kosteas, TUM Factor f(R) from Source II alu 2402.01.04 Training in Aluminium Application Technologies for Base Metal and Transverse Butt Weld The above mentioned result of S-1/S0 = 1.41, established on the basis of a rather large and homogeneous sample of small specimens, together with the almost identical value of S-1/S0 = 34.0/23.6 = 1.44 as calculated for the large welded components of the TUM aluminium beams, Figure 2402.01.05, lie in accordance with further minimum values as will be shown, and indicate thus the limit to be attained with some degree of reliability for welded details. Stress Range ∆σ [MPa] TUM welded beams EAA 3/89 (prt.2/Uhry) 100 R = -1 Serie 2 m = 2.8 R = 0.1 34.0 Serie 1 m = 2.7 23.6 10 104 105 106 2 5 107 Cycles to Failure alu Effect of R-Ratio on TUM Beam Tests of the 1982-1986 Training in Aluminium Application Technologies Research Program 2402.01.05 Stage III Evaluation Additional support in the case of welded beams came from test results of the current TUM beam test program 1987-1991. Valid statements based on a reliable number of test points for 7020 beams were possible in the case of longitudinal non-load-carrying fillet TALAT 2402 9
- 10. welds (web-to-flange welds with start and stop positions or tack welds) giving at 2.106 cycles f(R)=1.14 for R=+0.1 to -1 and f(R) = 1.57 for R = +0.6 to -1 and similarly in the case of transverse load-carrying fillet welds of flange attachments, i.e. cover plates f(R) = 1.24 for R = +0.1 to -1 and f(R) = 1.60 for R = +0.6 to -1. The fourth information source added significant weight to the evaluations by the considerable amount of small specimen data, almost 19000 data points, on base material and various weldments in the standard 5000, 6000 and 7000 alloy series. The following Figure 2402.01.06, Figure 2402.01.07 and Figure 2402.01.08 summarise minimum/mean/maximum enhancement factors f(R) at 2.106 cycles and between the R values 0 and -1. Especially for welded details, i.e. joints with assumed significant residual stresses, it was decided to accept an enhancement factor only in the range between 0 and -1. For values R > 0 the factor should be equal to one. alu Enhancement Factor f(R) at 2*106 Cycles 2402.01.06 Training in Aluminium Application Technologies for Base Material TALAT 2402 10
- 11. alu Enhancement Factor f(R) at 2*106 Cycles 2402.01.07 Training in Aluminium Application Technologies for Transverse Butt Weld alu Factor f(R) at 2*106 Cycles for Longitudinal or Transverse, Training in Aluminium Application Technologies Load-Carrying or Non-Load-Carrying Fillet Weld 2402.01.08 The Fatigue Workshop evaluations were completed by information on the treatment of the R-ratio effect on fatigue strength as these had been included in a recommendation and a standard for the design of aluminium structures. Figure 2402.01.09 and Figure 2402.01.10 give information from the proposal for the Aluminum Association in the U.S.. TALAT 2402 11
- 12. AA 8/1985 Sanders/Fisher (Olivier/Ritter 1979) 3 2.5 f(R) 2 1.5 1 -1 -0.5 0 0.5 1 R-Ratio butt weld, overfill cruciform, fillet plate with hole cruciform, full penetration alu Enhancement Factor f(R) in Design Recommendations Training in Aluminium Application Technologies Draft of the Aluminum Association - (a) 2402.01.09 AA 8/1985 Sanders/Fisher 3 2.5 f(R) 2 1.5 1 -2 -1.5 -1 -0.5 0 0.5 1 R-Ratio 5000 butt weld aluminium rivets aluminium bolts alu Enhancement Factor f(R) in Design Recommendations Training in Aluminium Application Technologies Draft of the Aluminum Association - (b) 2402.01.10 Figure 2402.01.11 and Figure 2402.01.12 attempt to reconstruct from rather limited information the scatter band of the factor f(R) for several welded details analysed and providing a background for the Italian standard on aluminium design. TALAT 2402 12
- 13. alu Mean Stress Amplitude Values at 2*106 Cycles for Training in Aluminium Application Technologies Several Welded Joint Types in 6000 and 7000 Alloys 2402.01.11 AA 5/85 after Atzori/Trendadue 1975 for 5000/6000 f(R) 3.5 3 3 2.5 2.4 2.1 2 1.9 1.6 2 1.5 1 1.2 1.3 1.3 1 Joint I Joint III Joint IV Joint VI Joint VII Joint Type extreme lower value extreme upper value D. Kosteas, TUM alu Extreme Limit Values for the Enhancement Factor f(R) for Training in Aluminium Application Technologies Several Welded Joint Types in 6000 and 7000 Alloys 2402.01.12 Drafting a Proposal for the Factor f(R) Using in general the mean values observed for the enhancement factor f(R) in all the cases outlined above a design proposal was drafted for the European Recommendations following the evaluations of the Workshops. The original proposal, as first suggested in Figure 2402.01.04, was now extended to include two practical cases for both base TALAT 2402 13
- 14. material elements and weldments, Figure 2402.01.13. In the one case knowledge of residual stresses in the structural element is available and if taken into account in the de- sign procedure allows for higher design stresses. Should no information on the stress situation be available or not considered in design then a lower line gives the respective values of f(R) vs. R for base material and weldments. The concept consists thus of two pairs of parallel lines each. The line for base material and residual stresses not known is not covered by actual data but based on an assumption following discussion on the Fatigue Workshop and a respective proposal by Dr. M. Ogle, The Welding Institute. Factor f(R) Sr(R)/Sr(+0.5) 1.9 I - base 1.6 I - weld 1.3 II - base II - weld I - II 1 -1 -0.5 0 0.5 1 R-Ratio I. residual stresses known II. residual stresses unknown Source:D. Kosteas, TUM Proposed Design Values for the Enhancement Factor alu 2402.01.13 Training in Aluminium Application Technologies after ERAAS Draft 8.6 In order to give a full picture of the final proposal and its rules as it was included in the ERAAS document the respective clauses are given in the Appendix. This may seem as a rather severe set of rules, departing also from the original position of the first evaluations. The introductory statements on residual stress measurement results should be considered very carefully, though. The existence and behaviour of residual stresses on larger elements under fluctuating loads is by no means quantifiable at the moment and an extrapolation of these results to every possible case in practice does not seem prudent. It must be born in mind that in the case of base material there was satisfactory experi- mental evidence available only in the form of small specimen tests, i.e. cases with "known" residual stress or equal to zero. The similar magnitude of strength ratios at a certain R value between larger components and small specimens seem to indicate that a fair amount of residual stresses may still be locked in the latter (this has also been shown by test results by Maddox and Webber a few years ago). Information about the specimen sizes, welding procedures and parameters would be necessary to clarify this matter, but were not available at the time of the above evaluations. TALAT 2402 14
- 15. To correctly read and apply values of the factor f(R) it should be mentioned once more that the diagram states only values relative to the fatigue strength at R = +0.5, the latter being the basic design value at 2.106 cycles of a specific structural detail relating to the classification or design curve value given in the data sheet of the Recommendations. Final ERAAS Design Proposal for f(R) The above proposal was discussed intensively, arguments concentrating on variability and scatter of enhancement factors f(R), the reliability of data sources, also their comparability, but above all on how accurate and realistic a definition of residual stress patterns can be in practice. Trying to cover these uncertainties it was decided to lower further the design proposal for the f(R) relationship, practically assuming now values justified by the majority of lower limits in the analysed data (as depicted for instance, but not exclusively, in Figure 2402.01.08, Figure 2402.01.09 and Figure 2402.01.10). Thus the proposal after Figure 2402.01.14 was adopted as the final design proposal for the European Recommendations. Factor f(R) = Sr(R) / Sr(+0.5) 1.6 I. Factor 1.3 II. III. 1 -1 -0.5 -0.25 0.5 1 R-Ratio I. Base / Wrought II. Connections III. Global residual stresses Source: Figure B1.1 ECCS ERAAS, 1992 alu R-Ratio Dependency and Residual Stresses (ERAAS) 2402.01.14 Training in Aluminium Application Technologies Line I is applicable only to base material and wrought products where there are no residual stresses acting on the structural elements or where such stresses can be fully taken into consideration in the design concept. Line II is to be used generally for all connections, also welded ones, where knowledge on the residual stress situation is available and is being considered. Line III covers those cases where significant global residual stresses are present but cannot be considered in the design analysis. This last case with no allowance for an enhancement factor includes thus all welded details in general practice. TALAT 2402 15
- 16. Residual Stress Effects We have already mentioned the difficulties in detecting, measuring or in any way quantifying the residual stress situation of a structural component. Indirectly this situation has been reflected in the proposal for the f(R) factor. Currently there are again some efforts undertaken to quantify the residual stress pattern of welded aluminium constructions. During the course of drafting the ERAAS information from the comprehensive welded beam fatigue testing programs at the Technical University of Munich it was possible to undertake initial residual stress measurements on full-size welded components of 7020 and 5083 alloys, Figure 2402.01.15. 0 B2 •10•27 0 12 0 B1 •10•24 40 0 0 12 C4 B2 12 00 C2 C1 40 0 B2 00 C3 4 0 B2 40 00 0 B1 12 40 0 40 B1 D2 15•30 0 00 40 0 0• 12 1 15 / E •350 40 0 E2 50•30 3 0 40 12 00 D1 300 • 5 0•1 15 40 0 40 0 B2 40 0 0 40 4 00 B1 0 40 00 12 00 12 Source: D. Kosteas, Technical University Munich alu Welded Aluminium Beams for Fatigue Tests 2402.01.15 Training in Aluminium Application Technologies The measurements themselves and the difficulties associated with the interpretation of these limited results or the sometimes somewhat contradictory information have been described elsewhere and allow presently only the following general conclusions: • residual stresses in welded components of considerable magnitude, reaching values up to the 0.2-yield-limit of the HAZ, was registered, Figure 2402.01.16 • scatter is an inherent feature in measurements made by the hole-drilling method. Efforts were undertaken to make measurements sufficiently close to the welds, approximately 1 mm off the weld toe, by using rosettes with the strain gages arranged on one side only • there were some but no significant differences in residual stresses in the structural details of the 7020 and 5083 alloy. TALAT 2402 16
- 17. HAZ yield strength design value 200 7020 R HAZ = 180 p0,2 150 5083 R HAZ = 125 p0,2 100 Residual Stress σz 50 in tension N/ mm2 0 B C1 C2 C3 C4 D1 D2 E V X X V V X 7020 5083 σx Structural Detail Designation according to ERAAS σ1 σz Residual Stress σ1 = from 1.20 to 1.60 σz Source: D. Kosteas, Technical University Munich alu Residual Stresses Measured in Fatigue Test Beams 2402.01.16 Training in Aluminium Application Technologies As seen in Figure 2402.01.16 the highest values of residual stresses were recorded at fillet welded longitudinal or transverse attachments on beam flanges. Residual stresses in these details attained values of over 180 MPa. Residual stress measurements at butt welded splices and cruciform joints made with butt-like full penetration welds attained values between 120 and 140 MPa. No answer can be offered for the time being to the question of whether initially measured residual stresses are maintained, and at what magnitude, during subsequent load cycling of the components. Indirect measurements at strain gauge monitored crack initiation sites showed values up to 120 MPa. these gauges may not have been sufficiently close to the maximum residual stress site, though. Residual stresses, therefore, may have been higher. The general lower location and steeper slope of S-N curves giving the behaviour of components vs. small specimen data agree with similar findings in steel weldments (see DIN 15018 and Eurocode 3 or ECCS TC6). There are still difficulties in interpreting differences between S-N curves with stress ratios of R = -1 and R = +0.1. The first show at times approximately 40% higher fatigue strength values of stress range plotted in a log-log diagram at 2.106 cycles. The effect is more pronounced in the case of 7020 alloy details. It does not seem prudent, though, to allow for a bonus in design values in such cases of large components, since sufficiently reliable data is still missing. TALAT 2402 17
- 18. Appendix B3.2 For the calculation of fatigue strength at values R other than +0.5 and N be- tween 1 104 and 5 106 cycles the fol- . . The following clauses from the ERAAS Fatigue Design, final version, December lowing procedure is given, assuming 1990, cover: that the basic design line as given in the Data Sheets is rotated around its value at 1 104 cycles. . B.3 Influence of R-Ratio For stress ratio values less than The resulting slope is: R=+0.5 a fatigue strength −2.301 enhancement factor f(R) may be m( R ) = considered and is given in Fig. 16. log f ( R ) + log ∆σ 2106 − log ∆σ104 ⋅ (see Figure 2402.01.14) This factor where is stated for a fatigue life N=2 106 . cycles. For other fatigue life values f(R): from Fig. 16 see Clause B.3.2. ∆σ2.106: the corresponding fatigue B3.1 The following cases shall be stress range of the basic design curve at 2 106 cycles (for R=+0.5). . distinguished (see Fig. 16): ∆σ104: the corresponding fatigue I Base material and wrought products stress range of the basic design in structural elements, assuming that curve at 1 104 cycles (for R=+0.5). . any residual stresses can be neglected for such elements For fatigue life values N > 5 106 . f(R) = 1.6 for R < -1 cycles the fatigue strength values of . f(R) = -0.4 R + 1.2 for -1≤R≤+0.5 design classes for welded details B, f(R) = 1 for R > +0.5 C, D, E, and F are defined assuming that the slope of the design curve is II Connections (welds or fasteners) in m'(R)=m(R)+2. For base material simple structural elements. design class A use m'(R)=m(R). f(R) = 1.3 for R < -1 . f(R) = -0.4 R + 0.9 for -1≤R≤-0.25 f(R) = 1 for R > -0.25 III For complex two- or three-dimensio- nal structures with residual stresses a constant factor shall be used f(R)=1 For connections in structures which have been adequately stress-relieved curve I shall be used TALAT 2402 18
- 19. 2402.02 Safety and Reliability • Reliability concept • Partial safety factor concept • Concept of fatigue design curves Values used in fatigue life predictions should be chosen so that they lead to a conservati- ve life. There are many different uncertainties which can influence fatigue life predicti- ons decisively. These may be associated for instance with − load estimation − stress calculation − S-N data − fabrication − damage accumulation theories For practical reasons the above influences will be expressed as safety margins within the design procedure expressing their inherent uncertainties. A fatigue design concept is based on an assessment of required life, cycles to failure, for the given environmental conditions and structural configuration. The assessment may be based on − reliability analysis − partial safety factors for loading and material related to respective S-N curve − fatigue design curves or 'allowable S-N curves' Reliability Concept The probability of failure of a structure can be determined through a suitable reliability theory, when the variability of the parameters governing fatigue life are known. So far as due to a certain load distribution S and a material or component strength distribution R a load-strength combination of the type R<S can occur a structure will fail (see Figure 2402.02.01). The probability distribution of the quantity R-S is then by definition the probability of failure (see Figure 2402.02.02). The safety factor is defined as the ratio of corresponding statistical values of the two original distributions. In Figure 2402.02.01 the definition of the partial safety factor for loading γS and the partial safety factor for resistance or material γR are given. The safety index β is related to the partial safety factors by the relation log γ S + log γ β= R (1) (s2 S +s 2 R ) TALAT 2402 19
- 20. Load and Resistance Distribution Probability Density log∆σR : fatigue strength f(Dse, se) 2 sR equivalent constant f(∆σ,sR) amplitude stress fatigue strength range distribution distribution se se SN SR SR = m log ∆σ e (log ∆σR + 2sR) log∆σ D. Kosteas, TUM alu Training in Aluminium Application Technologies Load and Resistance Distribution 2402.02.01 Probability Density standard deviation of failure curve: sR + s 2 2 e failure curve probability of failure f ( ∆σ R , sR ) − f ( ∆σ e , se ) β ⋅ sR + s 2 2 e log ∆σ (log ∆σ R + 2 ⋅ sR ) − log ∆σ e alu Probability of Failure Distribution 2402.02.02 Training in Aluminium Application Technologies Assuming that the S-N relationship is expressed by a straight line of slope m in log-log co-ordinates for a given life N we usually distinguish between • a the allowable loading for this life (see Figure 2402.02.03) line referring to the mean of fatigue strength ∆σ • a line referring to limit value of fatigue strength ∆σR and a distance of two standard deviations 2sR from the mean value as above - identical to the design classification value for a structural detail in the design recommendations • an 'amended' line in γm-fold distance and, lastly, • a line in a γl-fold distance from the last one representing. TALAT 2402 20
- 21. Schematic Definition of Safety Factors log ∆σ Stress Range 2sR β = sR + s 2 2 e γ mf log ∆σ R + 2sR = ∆σ f γL log ∆σ R γL "amended" class Cycles to Failure log N alu Training in Aluminium Application Technologies Schematic Definition of Safety Factors 2402.02.03 Following the usual definition of design lines in Recommendations as fatigue strength limits with 97.5% probability of survival and with respective partial safety factors equa- tion (1) can be written for the purposes of a fatigue assessment as follows log γ S + log γ + 2 sR β= R (2) ( sS2 + sR ) 2 This equation indicates the safety level, i.e. the probability of failure at the end of the design life. Taking as a basis a proposal of the Nordic committee the value of the index ß is in functional relationship with the annual probability of failure pf,1 (see Figure 2402.02.04) log(pf,1) = -0.4388 - 0.1767*β - 0.20908*β2 (3) This relation gives us the possibility to calculate recommended β-values for different applications and design lives of structures. As an example, BS8118: 1991, Part 1 indicates the following values (see also Figure 2404.02.05) Highway bridges 120 years Buildings, cladding 30 years Flood protection works 100 Boats 30 Buildings, primary structures 100 Cranes 20 Breakwaters 60 Containers 15 Lattice towers and masts 50 Vehicle bodies 10 Tall towers 50 Scaffolding 10 Railway vehicles 35 TALAT 2402 21
- 22. f, 1 curve estimate through logPf, 1 = - 0.4388 - 0.1767β - 0.20908β² β k S s S + log γ F + log γ M + k R s R β= 2 2 sS + sR alu Training in Aluminium Application Technologies Safety Index β 2402.02.04 Design Lives after BS 8118: 1991, Part 1 Type of Structure Design Lives in Years Highway Bridges 120 Flood protection works 100 Buildings, primary structures 100 Breakwaters 60 Lattice towers and masts 50 Tall towers 50 Railway vehicles 35 Buildings, cladding 30 Boats 30 Cranes 20 Containers 15 Vehicle bodies 10 Scaffolding 10 D. Kosteas, TUM alu Training in Aluminium Application Technologies Design Lives 2402.02.05 Equation (2) can be solved if the load and the fatigue strength distributions with respec- tive scatter values are known. There is only scant information about load distributions and an additional problem arises due to the fact of specific load histories and stress spectra in various applications. Recent comprehensive fatigue test analysis has provided TALAT 2402 22
- 23. several values for different aluminium alloys and their welded joints also in the case of large components, Figure 2402.02.06. The values in the diagram are logarithms of the standard deviation of the fatigue strength. For design purposes a transformation to respective values in terms of fatigue life can be derived SR,(logN) = m*SR,(log∆σ). Accordingly the relationship between the safety factors in the strength scale and the life scale would be logγ(log∆σ) = m*logγ(logN). Standard Deviations of Fatigue Strength sRlog∆σ TUM Beams Standard deviation of fatigue strength max value min (ECCS TC2 steel) all R-ratios pooled after Kosteas + Ondra "Safety & Reliability", INALCO ´95, Cleveland, OH, USA - 1995 Safety and Reliability - alu Standard Deviations of Fatigue Strengths 2402.02.06 Training in Aluminium Application Technologies As a result of the above difficulties in defining parameters for the described reliability assessment procedure, especially the definition of an appropriate probability of failure and respective β-value, this procedure is not yet a part of recommendations. We menti- on here the attempt to present certain definitions and values in the ECCS 6 'Fatigue De- sign of Steel Structures Recommendations' where a proposal of an appropriate value for β = 3.5 has been stated. Partial Safety Factor Concept It is obvious that a direct definition of recommended partial safety factor values presents the least difficulties for the engineer in practice. But even such a procedure has not been incorporated into recommendations in the case of fatigue design. It is already though a part of the static design assessment procedure, for instance Eurocode 3 Steel, ECCS 6 Recommendations for fatigue design in steel, ECCS 2 Recommendations for Aluminium Alloy Structures, BS 8118: 1991. TALAT 2402 23
- 24. In drafting the recent recommendations for aluminium design in fatigue values for the partial safety factors have been discussed in estimating design curves. As an indication for recommended values in this area the following is stated. For the fatigue material safety factor γR and depending on the consequences of failure or the redundancy of a structure the values of 1.2 (statically determinate structure) and 1.0 (statically indeterminate structure) in case of easy inspectability of the component for fatigue cracks is proposed. In case that components cannot be inspected the respective values are 1.4 and 1.2. The condition in the fatigue assessment procedure is that estimated life should not be shorter than the factored design life. Here the fatigue life safety factor γS,(logN) expres- ses the quality and confidence of the loading history. If records of loading are kept, or frequency of loading is well established γS(logN) = 1.25, but in the case that no records are kept or frequency is unknown a substantial increase of γS,(logN) = 10 is to be assumed. These values correspond to γS,(log∆σ) values of 1.08 and 2.15 respectively for a representative slope value of m = 3.75 as recorded in several details of the ERAAS Fatigue Design. Especially in reassessments of a structure in mid-life this factor should also be reassessed. Defining the product of the two partial safety factors as a nominal safety γ = γR,(log∆σ) *γS,(log∆σ) the following values result from the above proposals in the case of the ERAAS Fatigue Design and for an S-N curve slope of m = 3.75. Structure is statically Inspectability Loading known unknown indeterminate good 1.06 1.85 poor 1.27 1.85 determinate good 1.27 2.22 poor 1.48 2.59 In comparison to these the respective values of Eurocode 3 for steel structures and especially a 'non-fail-safe' structure (i.e. in the case that component failure results in a an overall failure are given: Inspect/Repair of Design Concept Design Concept component is fail safe non fail safe easy 1.00 1.25 difficult 1.15 1.35 It must be pointed out that the Eurocode postulates a defined pattern of maintenance and that in the case of difficulties with inspection and repair the owner should be notified. TALAT 2402 24
- 25. Concept of Fatigue Design Curves Current recommendations for fatigue design in aluminium alloy structures use the con- cept of design curves almost unanimously and do not make use of any further safety fac- tors. This is for instance the case with the 'ECCS-European Recommendations for Aluminium Alloys Fatigue Design' (1992) and the 'British Standard 8118: 1991 Structural Use of Aluminium'. The latter leave the possibility open for the designer to introduce additional partial safety factors for both loading and fatigue strength. The overall load factor γS should be taken to be unity provided that the loading and the evaluated fatigue strength data comply with certain conditions pertaining to loading. All sources of fluctuating stress in the structure should be identified and obtained as an up- per bound estimate of the service loading sequence for the structures design life. Reali- stic assessment of the fatigue loading is crucial to the calculation of the life of a structure. In both recommendations (ERAAS-Fatigue Design and BS 8118) the value of the partial safety factor on fatigue strength γR is assumed to be unity as well. The design curve through which the fatigue assessment is performed is defined at a „mean minus 2 standard deviation level“ below the mean line through experimental data. In certain circumstances the designer may wish to increase the nominal design life by multiplying by a factor (the fatigue life factor γS,(logN) > 1). The choice of the value of this factor could be influenced by the following conditions: • the possibility of increasing crack growth during the later stages of the life of the detail • the accuracy of the assumed loading spectrum • whether records of loading will be kept during the life of the detail • the possibility of a change of use of the structure in mid-life The designer may also wish to apply a fatigue material factor χR,(log∆σ) to the design stress range as given by the design curves in the recommendations. The design stress range would be divided by χR > 1 and the choice of the appropriate value could be in- fluenced by the following considerations: • the need for the detail to exist in a very hostile environment • whether failure of the detail will result in failure of the entire structure, or whether alternative load paths exist. The assumptions of the previous paragraph indicate recommended values. TALAT 2402 25
- 26. 2402.03 Background on Current Design Recommendations • European Recommendations ERAAS Fatigue Design 1992 − Full-size component testing and analysis − Detail classification and design curves − The S-N slope proposal − Comparison to steel codes • The British Standard 8118:1991 − Data sources − Data analysis and detail classification − Design curves − Classification of details • Comparison between BS 8118 and ERAAS Given the fact that currently the two most complete and extensive documents covering fatigue design of aluminium structures are the European Recommendations for Aluminium Alloy Structures Fatigue Design and the British Standard BS 8118 an outline of the drafting stages, the data analysis and evaluation and the ensuing design format is presented. This background information provides the necessary knowledge for adaptation of procedures in design problems with special environmental conditions or manufacturing parameters and possible utilisation of other specific experimental data. In the following paragraphs on the ERAAS description concentrates more on the data background and its analysis. The description on BS 8118 presents some basic considerations about fatigue specifications. The two documents show many similarities in the data evaluation and classification, a comparison is given in a third section. Finally the BS document gives also full details on quality assurance, but this is handled underTALAT Lecture 2404. European Recommendations ERAAS Fatigue Design 1992 Bearing in mind that in preparing the recommendations one of the most important items to be resolved was the definition of design values respective to specific structural details considerable consultations took place trying to pinpoint the type of details reliably supported by experimental evidence or the number of different ones to be considered in the document. Out of a total of over 45 different details mentioned in various specifications of the time it was recognised that information was available for only 14 of them. If one demanded statistically reliable data the number had to be reduced to a "nucleus" of 6 details. TALAT 2402 26
- 27. Full-Size Component Testing and Analysis The above elements were determinative of the actions to follow. Considering previous work of ECCS TC2 and corresponding to the interests of several national bodies the European Aluminium Association (EAA) decided in June 1988 to provide within the framework of the COST 506 Program of the Commission of European Communities a widely accepted information base for a standard on advanced structural design of aluminium components exposed to fatigue loading. The information base would include fatigue data related to full-scale components available in Europe by this date. Within the EAA a study was performed on "the data harmonisation and establishment of principles for a fatigue design code for welded aluminium structural elements" at the Technical University of Munich together with the Centre de Recherches Pechiney in Voreppe, France. The work plan, as outlined initially by the author, included: (1) establishment of a common data base, (2) establishment of analysis methodology, (3) establishment of cases to investigated, (4) statistical/regression analysis of individual data sets or "families"/groups of data sets, (5) definition of characteristic values, and (6) proposal for P-S-N curves for design along established concepts. This "COST 506 - EAA Study" provided the first comprehensive outline for the fatigue behaviour of structural components, especially beams, in aluminium. Later efforts concentrated on enlarging this data base through additions of further fatigue test results (TUM Beam Fatigue Project B), numerous additional attempts to compare sets of data, to analyse variations, to define influence of geometrical parameters, possible influence of alloy effect or residual stresses and R-ratio upon fatigue behaviour, to define structural detail classifications and to estimate design values. Figure 2402.03.01 outlines the range of materials and structural details covered by the various analyses and included in the final document of the ERAAS. THE COST 506 - EAA DATA PACKAGE Beams Source No. of No. of No. of Struct. Details Data Sets Data Points ALS 25 110 983 TUM 11 38 174 AMAG 8 11 90 Total Number of Data Points: 1247 including 142 run-outs Base Metal: 105 Data Points Weldments: 1142 Data Points Small Specimens ALS Structural No. of No. of Detail Data Sets Data Points Base Metal 11 423 Drilled Holes 3 123 Butt Weld Trans. 10 407 Total Number of Data Points: 953 ALS alloy 6005A tests only TALAT 2402 27
- 28. Recommendations Background Source COST/EAA LME/A*L 1989 1991 Core of data (LME-A*L) 10 alloys 7 alloys up to up to 35 details specimens Earlier CAFDEE 30 details standards 1986 No. of 3 alloys (LME-ISU) 6 details 3 alloy gr. 4 details ERAAS-Fatigue 5000 32 design details 6000 Al-Gr. grouped in 7000 19 different S-N lines Source: D. Kosteas, TUM alu Data Background of Design Recommendations 2402.03.01 Training in Aluminium Application Technologies Taking into account the views expressed above on the reliability of existing data packages and the respective analyses it was decided to take into account fatigue test data on aluminium components, beams, as base material and welded details. Only a few data were available in riveted connections or as notches in the form of drilled holes. Three institutions contributed to the respective data packages, as outlined in the above table. Because of the high degree of uniformity in a further data package concerning tests on small specimens with alloy 6005A and the comprehensive information on parameters such as plate thickness and stress ratio it was felt that these data would contribute decisively to the formulation of respective influences on fatigue and they were added to the analysis. Two parallel analysis procedures were undertaken, see boxes below, with corresponding statistical-regression models. The first used the initially "unidentified" data sets - i.e. distinguished only by their data set number but not described as to their corresponding structural detail type or other characteristics - in an attempt to prove the statistical compatibility of certain groupings of data or the fact that individual data sets could be reliably related to a common group leading thus to the "detail class" for design purposes. The second used the model to predict individual S-N relationships of both original data sets and "families" of data sets, deciding about the possible groupings primarily through engineering judgement - i.e. taking into account knowledge about structural detail type, failure location and type, initial imperfection, workmanship, alloy, joining procedure, etc. It should be pointed out that there was a very satisfactory correspondence between the end results of the two parallel analysis procedures - especially when considering the desired subsequent classification of design cases in a limited number of classes. TALAT 2402 28
- 29. Especially in the first analysis internal coherence of each group was carried out: characteristic values of data sets of each group were compared (scatters, slopes, logcycle means for a given stress level); within the groups data sets exhibit the same slope and scatter values; the significant differences between logcycle means of data sets are not "physically" too important, compared to data set scatter. THE COST 506 -EAA ANALYSIS PROCEDURE Analysis Uhry/CRV Analysis Kosteas/TUM (purely statistical) (engineering assumption) Individual Data Sets maximum likelyhood with or without run-outs censored data = run-outs maximum likelyhood with run-outs test for outliers test for outliers standard linear regression Data Sets Grouped grouping on the basis of common grouping on the basis of individual slope, intercept and scatter; same structural detail significantly different from respective group parameters (graphical verification) statistical analysis of each group = "family" For several reasons such as conservative analysis in view of limited or inexact information, difficulties in establishing run-outs from current reports or test procedures, further analysis options - beyond the maximum-likelyhood method exercised by both CRV and TUM - were carried out by TUM such as a linear regression excluding run- outs altogether and a linear regression assuming identified run-outs as failed specimens. THE COST 506 -EAA ANALYSIS MODELS Model (1) logN = a + b*logS double-log linear model for the analysis of individual data sets Model (2) logN = a(i) + b*logS assuming that one certain feature has no effect on scatter or slope but only on the intercept of the lines Model (3) logN = a(i) + g(j) + b*logS assuming that two features have no effect on scatter or slope but only an additive effect on the intercept of parallel lines TALAT 2402 29
- 30. The effects of alloy, R-ratio, plate thickness and data source were also investigated on subgroups of "balanced data" extracted from the global file of data sets in order to avoid confusions or bias. The alloy effect was studied on Alusuisse data only, since these comprised a comprehensive set of data, approximately equal numbers of observations for each alloy and involved a greater number of alloys (see boxes below). The study was carried out according to the following steps: a) a subfile was set-up containing those common details present for the different alloys, b) for each alloy the common slope and scatter values for the data sets of this alloy were estimated using the statistical model no. 2 (see box above) and supposing that here the data set had no effect on scatter or slope but only on the location of the parallel straight regression lines, c) scatters of different alloys were compared by the Hartley test, d) slopes were compared by the studentized range test, e) alloys were gathered and the alloy effect on logcycle mean was estimated using the statistical model no. 3 (see box above) and supposing that the alloy as well as the detail have no effect on slope or scatter and that their effects on the location of the regression lines are simply additive, i.e. they have no interaction. Three similar analyses were performed for the listed alloy groups. Summarising the results: no alloy effect was observed for the welded details, whereas in the case of parent material alloy 7020 exhibited higher values than the 5000 or 6000 series alloys with an estimated difference of d = 0.8 + or - 0.2 in logcycle mean for a stress level of 100 MPa. Alloy Effect Flange Edge 6082 Attachment with or without transition Radius Coverplate Flange Attachment, vertical, longitudinal 5086 Web Stiffener 6082 Web Attachment 6005A 7020 Butt Weld, transverse 5083, 5454 6005A, 6082 6082, 7020 Base Metal, Extrusions, Built-up Beams TALAT 2402 30
- 31. Thickness Effect Source Flanges Attachments ALS 10 8 to 10 TUM 15 110 or 15 AMAG 15 15 R-Ratio Effect Source 0,15 0,10 0,06-0,08 -1 ALS X X X TUM X X AMAG X The R-ratio effect was studied with the same methodology as above, but solely on TUM beam data since we had here consistent and sufficient data on 3 details: all data for alloy 7020 and in the two R-ratio values +0.1 and -1. The three details - longitudinal vertical attachment with fillet welds on beam flange, coverplate on built-up beam flange, full beam connection with butt weld with overfill as welded - showed non-significant differences in slope/scatter (-2.7/0.15 and -2.8/0.18 for the R-values +0.1 and -1, respectively), but exhibited a significant difference for the logcycle mean value at a stress of 100 MPa; here the value for R = +0.1 was 4.61 ± 0.07 and the value for R = -1 was 5.01 ± 0.07, i.e. a difference as correction between the two R-ratios of 0.4 ± 0.1. The effect of R-ratio has been studied later on in considerable depth, utilising further test results, and, especially the extensive contingent of small specimens of the Fatigue Workshop Zurich - see following chapters. Variations in the thickness of cross section elements of the beams and their attachments was not sufficiently significant so as to be quantitatively stated. Taking into account the above mentioned small specimen test results and bearing in mind the well established experience from earlier investigations of no significant thickness effects, at least for the range between 6 and 15 mm, the issue was not followed more closely. Finally, a possible effect of the data source was studied graphically. For six structural details no consistent pattern emerged for the relation of the three data sources. The same was valid when comparing logcycle mean values for a given stress value for details from the respective source. For the structural detail of transversely butt-welded beams results available from all three sources were compared as to significant differences in their scatter, slope or logcycle mean values. Differences were not significant. The overall conclusion was that results from the three sources were considered homogeneous enough to be analysed simultaneously as one data set. TALAT 2402 31
- 32. Detail Classification and Design Curves Following several in-between proposals the format of the recommendations was finalised and the concept discussed called for: − a set of S-N curves as representative design lines, limited in number, − lower limit curves, i.e. strictly "mean minus two standard deviations", thus covering most unknown variables in detail type, manufacturing, quality and loading parameters, − straight line regression, often extrapolated down to regions around 2*106 cycles, on the safe side, often rather conservative though, for a wide spectrum of applications of the recommendations, − a clause in the recommendations to enable more sophisticated design and manufacturing with considerably higher quality and ensuing fatigue strength. A second concept emerging was demanding for: − a more rigid design procedure with a greater number of structural details defined in more detail in the recommendations, − a larger number of variations of these details according to manufacturing characteristics (especially for weldments) with respective strength levels, demonstrating thus in a better way capabilities of the material, and − as a result this meant a larger number of detail classification cases and design lines. The above led to the decisions for the fatigue stress range value at 2 ⋅ 106 cycles of the basic design curve (R = +0.5). Information on the initial test values, R-influence factors and residual stress effects (TUM test reports, EAA evaluations, Workshop results) was integrated into proposals for the Recommendations. The "Data Sheet", Figure 2402.03.02, provides the link between the design curve and detail description in the Recommendations and the background information analyzed. It represents also a key- element for the implementation of the Aluminium Data Bank and the development of the ALFABET design procedure system, see Lecture 2404.01. A need for a more detailed and diversified classification of butt welds, depending on manufacturing quality was reached by enlarging the number of classes to and by re-analysing all available data in small specimens, extruded or built-up components. TALAT 2402 32
- 33. The ERAAS Fatigue Data Sheet Background Regressional S/N Plot of analysis experimental log∆S " """ " " data Linear analysis practically "" " " "" " " Influences by between 104 and 2 x 106 " """ ! ! ! source, alloy, logN = -m log∆σ + C " " !! " ! ! R-ratio or other parameters, and outliers,run-outs Reference to literature sources logN (EAA reports etc.) and AlDaBa Foreground Detail description Design log∆S S/N-Curve m Detail description pertaining to above experimental data and accompanied by manufacturing parameters with m' possible further remarks for strength enhancement logN alu Training in Aluminium Application Technologies The ERAAS Fatigue Data Sheet 2402.03.02 The S-N Slope Proposal Other than mere statistical aspects had to be considered for the definition of the design S-N lines. The degree of uniformity and harmonisation regarded as optimum under the implied or specified conditions has been attained mainly through best fit at the desired probability of survival level of fatigue strength at the critical life region, most times at 2 ⋅ 106 cycles, and an assumed slope value, common for a group of structural details. That these values lie within the range of experimentally established values is demonstrated with Figure 2402.03.03 showing the data point field of slope values m vs. fatigue strength for the data file of the COST 506 - EAA Study; with Figure 2402.03.04 showing the values for welded details for the TUM beam programs; and finally through Figure 2402.03.05 which gives the TUM welded beam slope values vs. their respective fatigue strength values at 105 cycles (since it is at this life region approximately that we have the centre of gravity of the data point field) against the assumed slope values at the three levels of m = 7.00 for parent material and m = 3.37 or 4.32 for the welded details. It should be mentioned perhaps that the above assumed slope values are in reality "calculated" values for two characteristic stress-life pairs from the respective S-N plots. This concept was checked against some other options, common in other specifications. The first option was to use instead of the fixed strength values (best-fit at critical lives) an equi-distant parallel design S-N line band with three possible, i.e. lying within the experimentally established values, slopes of m = 3.4 / 3.8 / 4.3. The second possibility was given by a parallel line band with m = 3.8 through the original ERAAS strength TALAT 2402 33
- 34. values at 2 ⋅ 106 cycles. The result of these comparisons showed clearly the advantages of the adopted ERAAS proposal. Source: D. Kosteas, TUM alu Slope vs. Fatigue Strength 2402.03.03 Training in Aluminium Application Technologies Source: D. Kosteas, TUM alu Slope V alues for TUM Welded Beams 2402.03.04 Training in Aluminium Application Technologies TALAT 2402 34

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment